Reduced cytotoxicity of insulin-immobilized CdS quantum dots using PEG as a spacer
© Selim et al; licensee Springer. 2011
Received: 18 July 2011
Accepted: 23 September 2011
Published: 23 September 2011
Cytotoxicity is a severe problem for cadmium sulfide nanoparticles (CSNPs) in biological systems. In this study, mercaptoacetic acid-coated CSNPs, typical semiconductor Q-dots, were synthesized in aqueous medium by the arrested precipitation method. Then, amino-terminated polyethylene glycol (PEG) was conjugated to the surface of CSNPs (PCSNPs) in order to introduce amino groups to the surface. Finally, insulin was immobilized on the surface of PCSNPs (ICSNPs) to reduce cytotoxicity as well as to enhance cell compatibility. The presence of insulin on the surface of ICSNPs was confirmed by observing infrared absorptions of amide I and II. The mean diameter of ICSNPs as determined by dynamic light scattering was about 38 nm. Human fibroblasts were cultured in the absence and presence of cadmium sulfide nanoparticles to evaluate cytotoxicity and cell compatibility. The results showed that the cytotoxicity of insulin-immobilized cadmium sulfide nanoparticles was significantly suppressed by usage of PEG as a spacer. In addition, cell proliferation was highly facilitated by the addition of ICSNPs. The ICSNPs used in this study will be potentials to be used in bio-imaging applications.
Keywordsnanoparticles immobilization polyethylene glycol insulin cytotoxicity
Recently, quantum dots [CdS, CdSe, ZnS, CdTe, etc.] (Q-dots) have attracted tremendous interest as luminescent probes in biological and medical researches due to their unique optical and chemical properties . Compared with traditional dyes and fluorescent proteins used as imaging probes, Q-dots have several advantages, such as tunable emission from visible to infrared wavelengths, broader excitation spectra, high quantum yield of fluorescence, strong brightness, photostability, and high resistance to photobleaching [2, 3]. However, the potential applications of Q-dots in biology and medicine have been limited due to their cytotoxic effects . Q-dots contain toxic components such as cadmium (from cadmium chalcogenide-based Q-dots) or lead (from lead chalcogenide-based Q-dots). Cd2+ and Pb2+ can be released from Q-dots, which would kill the cells . Therefore, to enhance stability, the surface modification of Q-dots is required. For example, biomedical applications require high-quality water soluble and non-toxic Q-dots. So far, numerous surface modifications of Q-dots have been explored, including the attachment of mercaptoacetic acid , mercaptopropionic acid , mercaptobenzoic acid , and biocompatible and chemically functionalizable inorganic shells, such as silica or zinc sulfide . All of these coatings can ensure the water solubility of Q-dots, but they are unable to enhance biocompatibility. Therefore, further coating with suitable water-soluble organic ligand/biomolecules is necessary to enhance the biocompatibility of Q-dots. To this end, Q-dots have been covalently linked with biorecognition molecules such as biotin , folic acid , peptides , bovine serum albumin , transferrin , antibodies , and DNA .
Polyethylene glycol (PEG) and its derivatives have been widely used as biomedical materials, such as drug delivery matrices and scaffolds for tissue engineering, due to their hydrophilicity, high solubility in aqueous and organic solvents, excellent biocompatibility, lack of toxicity and immunogenicity, and ease of excretion from living organisms. Among PEG derivatives, the most important one is amino-terminated PEG . On the other hand, insulin, which reduces blood glucose levels, is often used for treating diabetic patients. However, insulin also acts as a growth factor, inducing cell proliferation [18, 19]. It has been previously shown by research groups [18–21] that immobilized insulin stimulates cell growth more actively than free insulin. Therefore, introduction of PEG-insulin conjugate onto the surface of Q-dots through chemical bonding may confer the combined advantage of PEG and insulin. Introduction of PEG onto the surface of nanoparticles protects against unwanted agglomeration, makes them more biocompatible, and decreases their nonspecific intracellular uptake. On the contrary, insulin grafted onto the distal end of the PEG chain can enhance cells growth.
In this study, mercaptoacetic acid-coated cadmium sulfide nanoparticles (CSNPs), typical semiconductor Q-dots, were synthesized in aqueous medium by the arrested precipitation method at room temperature. Then, PEG with amino groups at both ends was reacted with carboxyl groups of CSNPs (PCSNPs) in order to introduce amino groups to the surface as well as to enhance biocompatibility. Finally, insulin was immobilized on the surface of PCSNPs (ICSNPs) to promote cell growth and further enhance biocompatibility. The surface properties of CSNPs and ICSNPs were characterized by X-ray diffraction (XRD), Fourier transform infrared (FT-IR) spectroscopy, transmission electron microphotography (TEM), and dynamic light scattering (DLS). Finally, human fibroblasts were cultured in the presence of nanoparticles to evaluate cell proliferation and cytotoxicity.
Preparation of mercaptoacetic acid-coated CdS quantum dots (CSNPs)
Water-soluble CSNPs were synthesized by following a previously published method . Briefly, carboxyl-stabilized CSNPs were synthesized by arrested precipitation at room temperature in aqueous solution using mercaptoacetic acid as the colloidal stabilizer. Nanocrystals were prepared from a stirred solution of 0.0456 g of CdCl2 (5 mM) in 40 ml of pure water. The pH was lowered to 2 with mercaptoacetic acid and then raised to 7 with 1 N NaOH. The mixture was deaerated by N2 bubbling for about 30 min, after which 40 ml of freshly prepared 5 mM Na2S (0.0480 g of Na2S in 40 ml of water) was added to the mixture with rapid stirring. The solution turned yellow shortly after the sulfide addition due to the formation of CSNPs (Scheme 1a in Additional file 1. CSNPs were separated from reaction by-products (sodium salt) via precipitation by the addition of acetone (4 ml of acetone per milliliter of nanocrystal solution). The precipitate was then isolated by centrifugation and dried in a freeze dryer. The prepared powder CSNPs were finally redispersed in water to obtain a clear colloidal solution with excellent stability (zeta potential, -66.65 mV). The free carboxylic acid groups of the prepared CSNPs are suitable for covalent coupling with the primary amino groups of various biomolecules.
Immobilization of insulin on the surface of CSNPs
Immobilization of insulin on CSNPs was performed in two steps. First, CSNPs were reacted with amino-terminated polyethylene glycol (PEG) to introduce amine groups on their surface. For this, CSNPs (0.2 g) were dissolved in aqueous solution (20 ml) containing 1-ethyl-3-(3-dimethylaminopropyl)carbodiimide (EDC) and stirred for 4 h to activate the carboxylic acid groups on the surface. Then, an excess amount of amine-terminated PEG was added to the solution, which was stirred for 24 h to obtain PEG-grafted CSNPs (PCSNPs) (Scheme 1b in Additional file 1). An excessive amount of PEG was used to suppress the crosslinking reaction on the surface and keep free amine groups at one end of the PEG chain after the reaction . Prepared PCSNPs were isolated via repeated centrifugation and finally dried in a freeze dryer. In the second step, insulin was immobilized on the surface of PCSNPs as follows: insulin was dissolved in phosphate buffer solution (2 mg/ml, pH 7.4) followed by the addition of a small amount of 0.1 N HCl. Then, 2% w/v water-soluble EDC and NHS were added to the solution, which was incubated at 4°C for 5 h to activate the carboxylic acid groups of the chain. Then, PCSNPs (5 mg/ml) were suspended in phosphate buffer solution (pH 7.4) with vortexing. This PCSNP suspension was mixed with the insulin aqueous solution and stirred gently overnight at room temperature to obtain insulin-immobilized PCSNPs (ICSNPs), as shown in Scheme 1 in Additional file 1. ICSNPs were isolated by repeated centrifugation and stored in phosphate-buffered saline (PBS) at pH 7. All conjugation reactions, unless otherwise noted, were carried out in the dark under a N2 ambient environment.
Fourier transform infrared (FT-IR) spectra were obtained using a JASCO FT-IR 300E spectrometer (JASCO Inc., Easton, MD, USA) at a resolution of 4 cm-1. Dried samples were ground with KBr powder and compressed into pellets for FT-IR examination. The samples were prepared by dropping the diluted nanoparticles on carbon-coated grids, followed by natural drying; then, the samples were observed by a transmission electron microphotograph (Philips CM 200 TEM; applied operation voltage, 120 kV; Philips Inc, Berlin, Germany. The hydrodynamic diameter and size distribution were determined by DLS by means of a standard laboratory-built light scattering spectrometer equipped with a BI 90 particle sizer (Brookhaven Instruments Corp., Holtsville, NY, USA). It had a vertically polarized incident light of 514.5 nm supplied by an argon ion laser (Lexel laser, model 95; Cambridge Lasers Laboratories Inc., Fremont, CA, USA. To investigate the crystal structure of CSNPs and bare CdS, XRD (RA/FR-571, Enraf Nonius, Deift, The Netherlands was used. The result was also compared with Joint Committee on Powder Diffraction Standards (JCPDS) file no. 10-454 to confirm whether or not any impurity phase exists in the CSNPs. The surface chemical composition was analyzed by electron spectroscopy for chemical analysis (ESCA, ESCA LAB VIG microtech, Mt 500/1, etc., East Grinstead, UK) with MgK α at 1, 253.6 eV and 150 W of power at the anode. A survey scan spectrum was taken, and the surface elemental compositions relative to the carbon were calculated from the peak heights, taking into account atomic sensitivity. The zeta potential is a very useful way of evaluating the stability of any colloidal system. In this study, the zeta potential was measured with a NicompTM 380 Zeta Potential (ZLS, Tokyo, Japan) employing the electrophoretic light scattering technique and using double-distilled water as a diluent.
In vitro cell behavior
MRC-5 human fibroblast cells (ATCC CCL, 171) were used in this experiment. Cells were routinely cultured at 37°C in a humidified atmosphere of 5% CO2 (in air) in a 75-cm2 flask containing 10 ml of Dulbecco's modified eagle medium (DMEM) supplemented with 10% fetal bovine serum (FBS) and 1% penicillin streptomycin G sodium. The medium was changed every 3 days. For subculture, the cells were washed twice with PBS and incubated with trypsin-ethylenediaminetetraacetic acid (EDTA) solution (0.25% trypsin, 1 mM EDTA) for 10 min at 37°C to detach the cells. The cells were washed twice by centrifugation and resuspended in DMEM media containing quantum dot nanoparticles, including CSNPs, PCSNPs, and ICSNPs (particle concentration, 0.2 mg/ml) for reseeding and growing in culture flasks. The cell density was fixed at 1 × 105 cells/ml. Cell morphologies were observed under a phase contrast microscope (Nikon Eclipse TS100, Tokyo, Japan) at predetermined time intervals.
The proliferation of fibroblasts cultured in the absence and presence of CSNPs, PCSNPs, and ICSNPs was determined by colorimetric immunoassay based on the measurement of 5-bromo-2-deoxyuridine (BrdU), which was incorporated during DNA synthesis [22, 23]. BrdU enzyme-linked immunosorbent assay (ELISA; Roche Molecular Biochemicals, Mannheim, Germany) was performed according to the manufacturer's instructions. Briefly, after 48 h of cell culture with CSNPs, PCSNPs, and ICSNPs in 24-well plates, the BrdU-labeling solution was added to each well and allowed to incorporate into the cells for an additional 20 h in a CO2 incubator at 37°C. Subsequently, the supernatant in each well was removed by pipetting. The cells were then washed twice with PBS and treated with 0.25% trypsin-EDTA (Gibco, Invitrogen, Tulsa, OK, USA) and harvested by centrifugation at 1, 000 rpm for 15 min. The harvested cells were mixed with a FixDenat solution to fix the cells and denature the DNA, followed by further incubation for 30 min. Subsequently, diluted anti-BrdU peroxidase (dilution ratio = 1:100) was added, and the cells were kept at 20°C for 120 min. After the removal of unbound antibody conjugates, 100 μl of substrate solution was added. The resulting mixture was allowed to stand for 20 min, and the reaction was completed by adding 1 M H2SO4 solution. The solution was then transferred to a 96-well plate and measured within 5 min at 450 nm with a reference wavelength of 690 nm using an ELISA plate reader.
To evaluate the cytotoxicity of Q-dots, the cells were separately cultured in a dish containing CSNPs, PCSNPs and ICSNPs and in a polystyrene culture dish alone. For qualitative observation, Live/Dead fluorescent staining with a LIVE/DEAD Cytotoxicity Kit (Biovision research products, Mountain view, CA 94043 USA) was used. Briefly, fibroblasts (3 × 104 cell/well) were seeded in a microplate with 1 ml of media containing CSNPs, PCSNPs, and ICSNPs (particle concentration = 0.1 mg/ml) without nanoparticles. After 2 and 4 days of incubation, the media were removed and the cells washed gently with PBS. Then, 0.3 ml of staining solution (prepared by mixing calcein-AM and propidium iodide with staining buffer at a concentration specified by Molecular Probes) was added to each well, and the plate was kept in an incubator for 15 min. Then, calcein/propidium iodide solution was removed, and the cells were washed once again with PBS. Finally, cells were viewed using a fluorescence microscope (FV-300, Olympus Co., Tokyo, Japan) coupled with a digital camera (FV-300, Olympus Co.). Live cells show green fluorescence images and dead cells show red images.
The cell viability experiment was performed in triplicate, and the results are expressed as mean ± standard deviation. Student's t test was employed to assess statistical significant difference of the results.
Results and discussion
Characterization of surface-modified CdS nanoparticles
Atomic percent of CSNPs, PCSNPs, and ICSNPs calculated from ESCA survey scan spectra
Atomic percent (%)
Insulin was immobilized onto the surface of mercaptoacetic acid-coated cadmium sulfide nanoparticles (CSNPs), and confirmation of insulin immobilization was carried out by FT-IR and ESCA. Size distribution of insulin-immobilized CSNPs (ICSNPs) having an average diameter of 13 nm as determined by TEM was narrow. The proliferation of fibroblasts was significantly increased by the presence of ICSNPs. ICSNPs also demonstrated lower cytotoxicity than CSNPs and PCSNPs. The ICSNPs used in this study will have potentials to be used in bio-imaging applications.
This work was supported by the Korea Ministry of Education, Science and Technology (contract no. 2009-0073282).
- Pan J, Feng SS: Targeting and imaging cancer cells by folate-decorated, quantum dots (QDs)-loaded nanoparticles of biodegradable polymers. Biomaterials 2009, 30: 1176. 10.1016/j.biomaterials.2008.10.039View ArticleGoogle Scholar
- Alivisatos AP, Gu WW, Larabell C: Quantum dots as cellular probes. Annual Review of Biomedical Engineering 2005, 7: 55. 10.1146/annurev.bioeng.7.060804.100432View ArticleGoogle Scholar
- Michalet X, Pinaud FF, L. Bentolila A, Tsay JM, Doose S, Li JJ: Quantum dots for live cells, in vivo imaging and diagnostics. Science 2005, 307: 538. 10.1126/science.1104274View ArticleGoogle Scholar
- Derfus AM, Chan WCW, Bhatia SA: Probing the cytotoxicity of semiconductor quantum dots. Nano Letters 2004, 4: 11. 10.1021/nl0347334View ArticleGoogle Scholar
- Yu WW, Chang E, Drezek R, Colvin VL: Water-soluble quantum dots for biomedical applications. Biochemical and Biophysical Research Communications 2006, 348: 781. 10.1016/j.bbrc.2006.07.160View ArticleGoogle Scholar
- Chen HM, Huang XF, Xu L, Xu J, Chen KJ, Feng D: Self-assembly and photoluminescence of CdS-mercaptoacetic clusters with internal structures. Superlattices and Microstructures 2000, 27: 1. 10.1006/spmi.1999.0794View ArticleGoogle Scholar
- Mitchell GP, Mirkin CA, Letsinger RL: Programmed assembly of DNA functionalized quantum dots. Journal of the American Chemical Society 1999, 121: 8122. 10.1021/ja991662vView ArticleGoogle Scholar
- Chen CC, Yet CP, Wang HN, Chao CY: Self-assembly of monolayers of cadmium selenide nanocrystals with dual color emission. Langmuir 1999, 15: 6845. 10.1021/la990165pView ArticleGoogle Scholar
- Chen F, Gerion D: Fluorescent CdSe/ZnS nanocrystal-peptide conjugates for long-term, nontoxic imaging and nuclear targeting in living cells. Nano Letters 2004, 4: 1827. 10.1021/nl049170qView ArticleGoogle Scholar
- Bruchez M Jr, Moronne M, Gin P, Weiss S, Alivisatos AP: Semiconductor nanocrystals as fluorescent biological labels. Science 1998, 28: 2013.View ArticleGoogle Scholar
- Chan WCW, Maxwell DJ, Gao X, Bailey RE, Han M, Nie S: Luminescent quantum dots for multiplexed biological detection and imaging. Current Opinion in Biotechnology 2002, 13: 40. 10.1016/S0958-1669(02)00282-3View ArticleGoogle Scholar
- Pinaud F, King D, Moore HP, Weiss S: Bioactivation and cell targeting of semiconductor CdSe/ZnS nanocrystals with phytochelatin-related peptides. Journal of the American Chemical Society 2004, 126: 6115. 10.1021/ja031691cView ArticleGoogle Scholar
- Hanaki KI, Momo A, Oku T, Komoto A, Maenosono S, Yamaguchi Y, Yamamoto K: Semiconductor quantum dot/albumin complex is a long-life and highly photostable endosome marker. Biochemical and Biophysical Research Communications 2003, 302: 496. 10.1016/S0006-291X(03)00211-0View ArticleGoogle Scholar
- Chan WCW, Nie S: Quantum dot bioconjugates for ultrasensitive nonisotopic detection. Science 1998, 281: 2016.View ArticleGoogle Scholar
- Goldman ER, Anderson GP, Tran PT, Mattoussi H, Charles PT, Mauro JM: Conjugation of luminescent quantum dots with antibodies using an engineered adaptor protein to provide new reagents for fluoroimmunoassays. Analytical Chemistry 2002, 74: 841. 10.1021/ac010662mView ArticleGoogle Scholar
- Gerion D, Parak WJ, Williams SC, Zanchet D, Micheel CM, Alivisatos AP: Electrophoretic and structural studies of DNA-directed Au nanoparticle groupings. Journal of the American Chemical Society 2002, 124: 11758. 10.1021/ja026166cView ArticleGoogle Scholar
- Wang L, Wang S, Bei JZ: Synthesis and characterization of macroinitiator-amino terminated PEG and poly(γ-benzyl-L-glutamate)-PEO-poly(γ-benzyl-L-glutamate) triblock copolymer. Polymers for Advanced Technologies 2004, 15: 617. 10.1002/pat.510View ArticleGoogle Scholar
- Hatakeyama H, Kikuchi A, Yamato M, Okano T: Influence of insulin immobilization to thermoresponsive culture surfaces on cell proliferation and thermally induced cell detachment. Biomaterials 2005, 26: 5167. 10.1016/j.biomaterials.2004.11.061View ArticleGoogle Scholar
- Kang IK, Cho SH, Shin DS, Yoon SC: Surface modification of polyhydroxyalkanoate films and their interaction with human fibroblasts. International Journal of Biological Macromolecules 2001, 28: 205. 10.1016/S0141-8130(00)00165-3View ArticleGoogle Scholar
- Kim EJ, Kang IK, Jang MK, Park YB: Preparation of insulin-immobilized polyurethanes and their interaction with human fibroblasts. Biomaterials 1998, 19: 239. 10.1016/S0142-9612(98)00203-8View ArticleGoogle Scholar
- Sasmazel HT, Aday S, Gumusderelioglu M: Insulin and heparin co-immobilized 3D polyester fabrics for the cultivation of fibroblasts in low-serum media. International Journal of Biological Macromolecules 2007, 41: 338. 10.1016/j.ijbiomac.2007.04.007View ArticleGoogle Scholar
- Maghni K, Nicolescu OM, Martin JG: Suitability of cell metabolic colorimetric assays for assessment of CD4+ T cell proliferation: comparison to 5-bromo-2-deoxyuridine (BrdU) ELISA. Journal of Immunological Methods 1999, 223: 185. 10.1016/S0022-1759(98)00220-8View ArticleGoogle Scholar
- Cui YL, Qi AD, Liu WG, Wang XH, Wang H, Ma DM, Yao KD: Biomimetic surface modification of poly(L-lactic acid) with chitosan and its effects on articular chondrocytes in vitro . Biomaterials 2003, 24: 3859. 10.1016/S0142-9612(03)00209-6View ArticleGoogle Scholar
- Smith NV: X-Ray Powder Data Files. Philadelphia: American Society for Testing and Materials; 1967.Google Scholar
- Pucci A, Boccia M, Galembeck F, Leite CAP, Tirelli N, Ruggeri G: Luminescent nanocomposites containing CdS nanoparticles dispersed into vinyl alcohol based polymers. Reactive and Functional Polymers 2008, 68: 1144. 10.1016/j.reactfunctpolym.2008.03.007View ArticleGoogle Scholar
- Wang Q, Kuo YC, Wang Y, Shin G, Ruengruglikit C, Huang Q: Luminescent properties of water-soluble denatured bovine serum albumin-coated CdTe quantum dots. The Journal of Physical Chemistry B 2006, 110: 16860. 10.1021/jp062279xView ArticleGoogle Scholar
- ASTM Designation F316–86: Standard test methods for pore size characteristics of membrane filters by bubble point and mean flow pore test. 752–757.Google Scholar
- Kuo YC, Wang Q, Ruengruglikit C, Yu H, Huang Q: Antibody-conjugated CdTe quantum dots for Escherichia coli detection. The Journal of Physical Chemistry C 2008, 112: 4818. 10.1021/jp076209hView ArticleGoogle Scholar
- Chowdhury PS, Ghosha P, Patra A: Study of photophysical properties of capped CdS nanocrystals. Journal of Luminescence 2007, 124: 327. 10.1016/j.jlumin.2006.04.001View ArticleGoogle Scholar
- Selim KMK, Lee JH, Kim SJ, Xing Z, Chang Y, Guo H, Kang IK: Surface modification of magnetites using maltotrionic acid and folic acid for molecular imaging. Macromolecular Research 2006, 14: 646. 10.1007/BF03218738View ArticleGoogle Scholar
- Chen G, Ito Y, Imanishi Y: Mitogenic activities of water-soluble and -insoluble insulin conjugates. Bioconjugate Chemistry 1997, 8: 106. 10.1021/bc960068xView ArticleGoogle Scholar
- Li JS, Ito Y, Zheng J, Takahashi T, Imanishi Y: Enhancement of artificial juxtacrine stimulation of insulin by co-immobilization with adhesion factors. Journal of Biomedical Materials Research Part A 1997, 37: 190. 10.1002/(SICI)1097-4636(199711)37:2<190::AID-JBM7>3.0.CO;2-MView ArticleGoogle Scholar
- Selim KMK, Xing ZC, Guo H, Kang IK: Immobilization of lactobionic acid on the surface of cadmium sulfide nanoparticles and their interaction with hepatocytes. Journal of Materials Science: Materials in Medicine 2009, 20: 1945. 10.1007/s10856-009-3741-1Google Scholar
- Selim KMK, Guo H, Kang IK: Albumin-conjugated cadmium sulfide nanoparticles and their interaction with KB cells. Macromolecular Research 2009, 17: 403. 10.1007/BF03218881View ArticleGoogle Scholar
- Maysinger D, Lovric J, Eisenberg A, Savic R: Fate of micelles and quantum dots in cells. European Journal of Pharmaceutics and Biopharmaceutics 2007, 65: 270. 10.1016/j.ejpb.2006.08.011View ArticleGoogle Scholar
- Gupta AK, Berry C, Gupta M, Curtis A: Receptor-mediated targeting of magnetic nanoparticles using insulin as a surface ligand to prevent endocytosis. IEEE Transactions on Nanobioscience 2003, 2: 255. 10.1109/TNB.2003.820279View ArticleGoogle Scholar
- Fischer D, Li YX, Ahlemeyer B, Krieglstein J, Kissel T: In vitro cytotoxicity testing of polycations: influence of polymer structure on cell viability and hemolysis. Biomaterials 2003, 24: 1121. 10.1016/S0142-9612(02)00445-3View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.